Carbon-fiber-reinforced polymer, carbon-fiber-reinforced plastic or carbon-fiber reinforced thermoplastic (CFRP, CRP, CFRTP or often simply carbon fiber), is an extremely strong and light fiber-reinforced polymer which contains carbon fibers. The polymer is most often epoxy, but other polymers, such as polyester, vinyl ester or nylon, are sometimes used. The composite may contain other fibers, such as aramid e.g. Kevlar, Twaron, aluminium, or glass fibers, as well as carbon fiber. The strongest and most expensive of these additives, carbon nanotubes, are contained in some primarily polymer baseball bats, car parts and even golf clubs where economically viable. Carbon fiber is commonly used in the transportation industry; normally in cars, boats and trains.
Although carbon fiber can be relatively expensive, it has many applications in aerospace and automotive fields, such as Formula One. The compound is also used in sailboats, rowing shells, modern bicycles, and motorcycles, where its high strength-to-weight ratio and very good rigidity is of importance. Improved manufacturing techniques are reducing the costs and time to manufacture, making it increasingly common in small consumer goods as well, such as certain ThinkPads since the 600 series, tripods, fishing rods, hockey sticks, paintball equipment, archery equipment, tent poles, racquet frames, stringed instrument bodies, drum shells, golf clubs, helmets used as a paragliding accessory and pool/billiards/snooker cues.
The material is also referred to as graphite-reinforced polymer or graphite fiber-reinforced polymer (GFRP is less common, as it clashes with glass-(fiber)-reinforced polymer). In product advertisements, it is sometimes referred to simply as graphite fiber for short.
Carbon-fiber-reinforced polymers are composite materials. In this case the composite consists of two parts; a matrix and a reinforcement. In CFRP the reinforcement is carbon fiber, which provides the strength. The matrix is usually a polymer resin, such as epoxy, to bind the reinforcements together. Because CFRP consists of two distinct elements, the material properties depend on these two elements.
The reinforcement will give the CFRP its strength and rigidity; measured by Stress (mechanics) and Elastic modulus respectively. Unlike isotropic materials like steel and aluminum, CFRP has directional strength properties. The properties of CFRP depend on the layouts of the carbon fiber and the proportion of the carbon fibers relative to the polymer.
The process by which most carbon-fiber-reinforced polymer is made varies, depending on the piece being created, the finish (outside gloss) required, and how many of this particular piece are going to be produced. In addition, the choice of matrix can have a profound effect on the properties of the finished composite.
One method of producing graphite-epoxy parts is by layering sheets of carbon fiber cloth into a mold in the shape of the final product. The alignment and weave of the cloth fibers is chosen to optimize the strength and stiffness properties of the resulting material. The mold is then filled with epoxy and is heated or air-cured. The resulting part is very corrosion-resistant, stiff, and strong for its weight. Parts used in less critical areas are manufactured by draping cloth over a mold, with epoxy either preimpregnated into the fibers (also known as pre-preg) or "painted" over it. High-performance parts using single molds are often vacuum-bagged and/or autoclave-cured, because even small air bubbles in the material will reduce strength.
For simple pieces of which relatively few copies are needed, (1–2 per day) a vacuum bag can be used. A fiberglass, carbon fiber or aluminum mold is polished and waxed, and has a release agent applied before the fabric and resin are applied, and the vacuum is pulled and set aside to allow the piece to cure (harden). There are two ways to apply the resin to the fabric in a vacuum mold. One is done manually and called a wet layup, where the two-part resin is mixed and applied before being laid in the mold and placed in the bag. The other one is done by infusion, where the dry fabric and mold are placed inside the bag while the vacuum pulls the resin through a small tube into the bag, then through a tube with holes or something similar to evenly spread the resin throughout the fabric. Wire loom works perfectly for a tube that requires holes inside the bag. Both of these methods of applying resin require hand work to spread the resin evenly for a glossy finish with very small pin-holes. A third method of constructing composite materials is known as a dry layup. Here, the carbon fiber material is already impregnated with resin (prepreg) and is applied to the mold in a similar fashion to adhesive film. The assembly is then placed in a vacuum to cure. The dry layup method has the least amount of resin waste and can achieve lighter constructions than wet layup. Also, because larger amounts of resin are more difficult to bleed out with wet layup methods, prepreg parts generally have fewer pinholes. Pinhole elimination with minimal resin amounts generally require the use of autoclave pressures to purge the residual gases out.
A quicker method uses a compression mold. This is a two-piece (male and female) mold usually made out of fiberglass or aluminum that is bolted together with the fabric and resin between the two. The benefit is that, once it is bolted together, it is relatively clean and can be moved around or stored without a vacuum until after curing. However, the molds require a lot of material to hold together through many uses under that pressure.
For difficult or convoluted shapes, a filament winder can be used to make pieces.
Manufacturers of carbon fibers
Major manufacturers of the commercial carbon fibers used for reinforcement include Hexcel, SGL Carbon, Toho Tenax, Toray Industries and Zoltek. Manufacturers typically make different grades of fibers for different applications.
Many carbon-fiber-reinforced polymer parts are created with a single layer of carbon fabric that is backed with fiberglass. A tool called a chopper gun is used to quickly create these composite parts. Once a thin shell is created out of carbon fiber, the chopper gun cuts rolls of fiberglass into short lengths and sprays resin at the same time, so that the fiberglass and resin are mixed on the spot. The resin is either external mix, wherein the hardener and resin are sprayed separately, or internal mixed, which requires cleaning after every use.
The primary element of CFRP is a fiber. From these fibers, a unidirectional sheet is created. These sheets are layered onto each other in a quasi-isotropic layup, e.g. 0°, +60° or −60° relative to each other. From the elementary fiber, a bidirectional woven sheet can be created, i.e. a twill with a 2/2 weave.
|This section does not cite any references or sources. (July 2008)|
Carbon-fiber-reinforced polymer is used extensively in high-end automobile racing. The high cost of carbon fiber is mitigated by the material's unsurpassed strength-to-weight ratio, and low weight is essential for high-performance automobile racing. Racecar manufacturers have also developed methods to give carbon fiber pieces strength in a certain direction, making it strong in a load-bearing direction, but weak in directions where little or no load would be placed on the member. Conversely, manufacturers developed omnidirectional carbon fiber weaves that apply strength in all directions. This type of carbon fiber assembly is most widely used in the "safety cell" monocoque chassis assembly of high-performance racecars.
Cast vinyl has also been used in automotive applications for aesthetics, as well as heat and abrasion resistance. Most top-of-the-line cast vinyl materials such as 3M's DiNoc (interior use) and SI's Si-1000 3D (exterior use) have lifespans of 10+ years when installed correctly.
Until recently, the material has had limited use in mass-produced cars because of the expense involved in terms of materials, equipment, and the relatively limited pool of individuals with expertise in working with it. Recently, several mainstream vehicle manufacturers have started to use CFRP in everyday road cars.
Use of the material has been more readily adopted by low-volume manufacturers who used it primarily for creating body-panels for some of their high-end cars due to its increased strength and decreased weight compared with the glass-reinforced polymer they used for the majority of their products.
Use of carbon fiber in a vehicle can appreciably reduce the weight and hence the size of its frame. This will also facilitate designers' and engineers' creativity and allow more in-cabin space for commuters.
Civil engineering applications
Carbon-fiber-reinforced polymer (CFRP) has become a notable material in structural engineering applications. Studied in an academic context as to its potential benefits in construction, it has also proved itself cost-effective in a number of field applications strengthening concrete, masonry, steel, cast iron, and timber structures. Its use in industry can be either for retrofitting to strengthen an existing structure or as an alternative reinforcing (or prestressing) material instead of steel from the outset of a project.
Retrofitting has become the increasingly dominant use of the material in civil engineering, and applications include increasing the load capacity of old structures (such as bridges) that were designed to tolerate far lower service loads than they are experiencing today, seismic retrofitting, and repair of damaged structures. Retrofitting is popular in many instances as the cost of replacing the deficient structure can greatly exceed its strengthening using CFRP.
Applied to reinforced concrete structures for flexure, CFRP typically has a large impact on strength (doubling or more the strength of the section is not uncommon), but only a moderate increase in stiffness (perhaps a 10% increase). This is because the material used in this application is typically very strong (e.g., 3000 MPa ultimate tensile strength, more than 10 times mild steel) but not particularly stiff (150 to 250 GPa, a little less than steel, is typical). As a consequence, only small cross-sectional areas of the material are used. Small areas of very high strength but moderate stiffness material will significantly increase strength, but not stiffness.
CFRP can also be applied to enhance shear strength of reinforced concrete by wrapping fabrics or fibers around the section to be strengthened. Wrapping around sections (such as bridge or building columns) can also enhance the ductility of the section, greatly increasing the resistance to collapse under earthquake loading. Such 'seismic retrofit' is the major application in earthquake-prone areas, since it is much more economic than alternative methods.
If a column is circular (or nearly so) an increase in axial capacity is also achieved by wrapping. In this application, the confinement of the CFRP wrap enhances the compressive strength of the concrete. However, although large increases are achieved in the ultimate collapse load, the concrete will crack at only slightly enhanced load, meaning that this application is only occasionally used.
Specialist ultra-high modulus CFRP (with tensile modulus of 420 GPa or more) is one of the few practical methods of strengthening cast-iron beams. In typical use, it is bonded to the tensile flange of the section, both increasing the stiffness of the section and lowering the neutral axis, thus greatly reducing the maximum tensile stress in the cast iron.
When used as a replacement for steel, CFRP bars could be used to reinforce concrete structures, however the applications are not common.
CFRP could be used as prestressing materials due to their high strength. The advantages of CFRP over steel as a prestressing material, namely its light weight and corrosion resistance, should enable the material to be used for niche applications such as in offshore environments. However, there are practical difficulties in anchorage of carbon fiber strands and applications of this are rare.
In the United States, prestressed concrete cylinder pipes (PCCP) account for a vast majority of water transmission mains. Due to their large diameters, failures of PCCP are usually catastrophic and affect large populations. Approximately 19,000 miles of PCCP have been installed between 1940 and 2006. Corrosion in the form of hydrogen embrittlement has been blamed for the gradual deterioration of the prestressing wires in many PCCP lines. Over the past decade, CFRPs have been utilized to internally line PCCP, resulting in a fully structural strengthening system. Inside a PCCP line, the CFRP liner acts as a barrier that controls the level of strain experienced by the steel cylinder in the host pipe. The composite liner enables the steel cylinder to perform within its elastic range, to ensure the pipeline's long-term performance is maintained. CFRP liner designs are based on strain compatibility between the liner and host pipe.
CFRP is a more costly material than its counterparts in the construction industry, glass fiber-reinforced polymer (GFRP) and aramid fiber-reinforced polymer (AFRP), though CFRP is, in general, regarded as having superior properties.
Much research continues to be done on using CFRP both for retrofitting and as an alternative to steel as a reinforcing or prestressing material. Cost remains an issue and long-term durability questions still remain. Some are concerned about the brittle nature of CFRP, in contrast to the ductility of steel. Though design codes have been drawn up by institutions such as the American Concrete Institute, there remains some hesitation among the engineering community about implementing these alternative materials. In part, this is due to a lack of standardization and the proprietary nature of the fiber and resin combinations on the market.
Carbon-fiber-reinforced polymer has found use in sports equipment such as racing bicycles. For the same strength, a carbon fiber frame weighs less than a bicycle tubing of steel, aluminum, or titanium. The choice of carbon-fiber weave can be carefully selected to maximize stiffness and minimize the chance of failure. The variety of shapes it can be built into has further increased stiffness and also allowed aerodynamic considerations into tube profiles. Carbon-fiber-reinforced polymer frames, forks, handlebars, seatposts, and crank arms are becoming more common on medium- and higher-priced bicycles.
While carbon-fiber frames and components can be both lighter and stiffer than those made of traditional metals, under some circumstances they have shown significant rates of cracking and failure. This can occur as because of a collision, but if components are overtorqued or improperly installed, cracking and failure can also result. It is possible for broken carbon frames to be repaired.
Other sporting goods applications include rackets, fishing rods, longboards, and rowing shells. The large majority of NHL ice hockey players use carbon-fiber sticks. Modern Pole vaulting poles are made of Carbon-fiber. Amputee athletes like Oscar Pistorius use carbon fiber blades for running.
This material is used when manufacturing squash, tennis and badminton racquets. Carbon-graphite spars are used on the frames of some sport kites and in the manufacture of high quality arrows for archery. Shoe manufacturers use carbon fiber as a shank plate in some basketball sneakers to keep the foot stable. It usually runs the length of the shoe just above the sole and is left exposed in some areas, usually in the arch.
In 2006, a company introduced cricket bats with a thin carbon-fiber layer on the back which were used in competitive matches by high-profile players (e.g. Ricky Ponting and Michael Hussey). The carbon fiber was claimed to increase the durability of the bats, however they were banned from all first-class matches by the ICC in 2007.
Due to its high ratio of strength to weight, CFRP is widely used in micro air vehicles (MAVs). In the MAVSTAR Project, the CFRP structures reduce the weight of the MAV significantly. In addition, the high stiffness of the CFRP blades overcome the problem of collision between blades under strong wind.
Especially aircraft of the sub-category of microlights (SSDR) take advantage of CFRP. Those aircraft, such as the E-Go, must comply with a weight less than 115 kg (254 lb) without fuel and pilot. Creating an aircraft of this class without the usage of CFRP would be extremely difficult.
CFRP has also found application in the construction of high-end audio components such as turntables and loudspeakers, again due to its stiffness.
It is used for parts in a variety of musical instruments, including violin bows, guitar pick-guards, and a durable ebony replacement for bagpipe chanters. It is also used to create entire musical instruments such as Viktorian Guitars carbon fiber rider models, Luis and Clark carbon fiber cellos, and Mix carbon fiber mandolins.
In firearms it can substitute for metal, wood, and fiberglass in many areas of a firearm in order to reduce overall weight. However, while it is possible to make the receiver out of synthetic material such as carbon fiber, many of the internal parts are still limited to metal alloys as current reinforced plastics are unsuitable replacements.
CFRP is used, either as standard equipment or in aftermarket parts, in high-performance radio-controlled vehicles and aircraft, e.g. for the main rotor blades of radio controlled helicopters—which should be light and stiff to perform fast aerobatic maneuvers.
Fire resistance of polymers or thermoset composites is significantly improved if a thin layer of carbon fibers is molded near the surface—dense, compact layer of carbon fibers efficiently reflects heat.
IBM/Lenovo's ThinkPad laptops, Dell's XPS13 and several Sony laptop models use this technology.
Carbon fiber is a popular material to form the handles of high-end knives.
End of useful life/recycling
|This section does not cite any references or sources. (June 2012)|
Carbon-fiber-reinforced polymers (CFRPs) have a long service lifetime when protected from the sun. When it is time to decommission CFRPs, they cannot be melted down in air like many metals. When free of vinyl (PVC or polyvinyl chloride) and other halogenated polymers, CFRPs can be thermally decomposed via thermal depolymerization in an oxygen-free environment. This can be accomplished in a refinery in a one-step process. Capture and reuse of the carbon and monomers is then possible. CFRPs can also be milled or shredded at low temperature to reclaim the carbon fiber, however this process shortens the fibers dramatically. Just as with downcycled paper, the shortened fibers cause the recycled material to be weaker than the original material. There are still many industrial applications that do not need the strength of full-length carbon fiber reinforcement. For example, chopped reclaimed carbon fiber can be used in consumer electronics, such as laptops. It provides excellent reinforcement of the polymers used even if it lacks the strength-to-weight ratio of an aerospace component.
Despite its high initial strength-to-weight ratio, one structural limitation of CFRP is its lack of a fatigue endurance limit. As such, failure cannot be theoretically ruled out from a high enough number of stress cycles. By contrast, steel and certain other structural metals and alloys do have an estimable fatigue endurance limit. Because of the complex failure modes of such composites, the fatigue failure properties of CFRP are difficult to predict. As a result, when utilizing CFRP for critical cyclic-loading applications, engineers may need to employ considerable strength safety margins to provide suitable component reliability over a sufficiently long service life.
Carbon nanotube reinforced polymer (CNRP)
In 2009, Zyvex Technologies introduced carbon nanotube-reinforced epoxy and carbon prepregs. Carbon nanotube reinforced polymer (CNRP) is several times stronger and tougher than CFRP and was used in the Lockheed Martin F-35 Lightning II as a structural material for aircraft.
- Gullapalli, Sravani and Wong, Michael S. (May 2011). "Nanotechnology: A Guide to Nano-Objects". Chemical Engineering Progress: 28–32.
- Kopeliovich, Dmitri. Carbon Fiber Reinforced Polymer Composites. substech.com
- Basic Properties of Reference Crossply Carbon-Fiber Composite. Oak Ridge National Laboratory (February 2000)
- Ismail, N. "Strengthening of bridges using CFRP composites." Beijing, 217–224.
- Rahman, S. (November 2008). "Don’t Stress Over Prestressed Concrete Cylinder Pipe Failures ". Opflow Magazine, American Water Works Association: 10–15
- "The Perils of Progress". Retrieved February 16, 2013. Bicycling Magazine, January 16, 2012
- "Busted Carbon blog". Retrieved February 16, 2013. Bustedcarbon.com
- "Carbon Bicycle and Component Care". Retrieved February 16, 2013. BicycleWarehouse.com
- "Inside Calfee Design's Carbon Repair Service". Bicycling Magazine. Retrieved February 16, 2013.
- "ICC and Kookaburra Agree to Withdrawal of Carbon Bat". NetComposites. 2006-02-19. Retrieved 2010-12-31.
- Zhao, Z. and Gou, J. (2009). "Improved fire retardancy of thermoset composites modified with carbon nanofibers". Sci. Technol. Adv. Mater. (free downloaddoi:10.1088/1468-6996/10/1/015005.) 10: 015005.
- Epovex press release (October 2009) "Zyvex Performance Materials Launch Line of Nano-Enhanced Adhesives that Add Strength, Cut Costs""Zyvex Materials Press Release"
- Trimble, Stephen (2011-06-26) "Lockheed Martin reveals F-35 to feature nanocomposite structures." Flight International.
|Wikimedia Commons has media related to: Carbon fiber reinforced plastic|
- Japan Carbon Fiber Manufacturers Association (English)
- Carbon fiber information from the Department of Polymer Science at University of Southern Mississippi
- Article on the basis of Carbon Fiber
- Engineers design composite bracing system for injured Hokie running back Cedric Humes
- The New Steel a 1968 Flight article on the announcement of carbon fiber
- Carbon Fibres – the First Five Years A 1971 Flight article on carbon fiber in the aviation field